EXPERIMENTAL INVESTIGATION INTO THE EFFECT OF GAS TUNGSTEN ARC WELDING ON Ti-6Al-4V
1professor in VNR vignan jyoti institute of technology, bachupally
2post graduate in VNR vignan jyoti institute of technology , bachuplly Email: 1Ravirajmani1970@gmail.com, email@example.com
ABSTRACT- An experimental investigation of enhancing mechanical properties of pulsed and non pulsed frequencies like 2, 4, 6, 8 using Gas Tungsten Arc Welding on Ti-6Al- 4V is presented. Butt welding of 2mm thickness titanium sheets is prepared by TIG Welding using argon gas as shielding gas.
Evaluating weld ability of Ti-6Al-4V by
welding conditions such as welding pass, amount of shielding gas and welding time interval is done. Experimentswere performed on titanium using destructive, non destructive tests and tensile tests are done so as to determine the ultimate tensile strength, yield strength and % elongation.
Index Terms –Welding, NDT, Shielding gas, Titanium
Welding of titanium structures is a cost effective manufacturing methods for numerous components used in aerospace applications.
Titanium has high specific strength and excellent corrosion resistance and is extensively used in aerospace, missiles and marine applications.
Titanium grade 5 is the most commonly used alloy which is considered to be alpha-beta alloy The dual phase, i.e. alpha + beta alloys offer a combination of excellent ductility and strength when proper heat treatment is given, which makes them stronger than alpha-phase and beta- phase. With the increased use of Ti, the joining of titanium has become more and more important. Welding of titanium alloy is difficult because titanium is chemically reactive at high temperatures. The studies have shown that during welding, titanium alloys pick up oxygen and nitrogen from the atmosphere easily .With the development of titanium in industries, Tungsten Inert Gas (TIG) welding is the most commonly used welding method for titanium.
The welded joint significantly affects the mechanical properties of the welded zone depending on the welding materials, welding conditions and welding environment. Like most titanium alloys, Grade 5 has outstanding
resistance to corrosion in most natural and many industrial process environments.
In this experimental investigation Ti-6Al-4V i.e., four number titanium grade 5 sheets of 150
300 dimension and thickness of about 2 are taken. They are subjected to Gas tungsten arc welding.
1. Ti sheets
Titanium gr-5 sheets are rarely available. They are cut according to the dimension mentioned by wire cut EDM carefully .No. of sheets used for welding are four.
2. Filler metal
For welding titanium Gr-5 of 2mm thickness by TIG welding process, a filler metal must be used and its composition is usually matched to the grade of titanium being weld. Filler metal in straight length with 150 long and 2 diameter was used for the experiment.
3. Shielding gas
Usually argon and helium are used for shielding in welding titanium. Argon is more widely used, since it is readily available and less costly. In this study Argon is used as shielding gas with flow rate at 10L/min.
4 Joint preparation :
Since the welding was carried out outside the welding chamber, without using travelling cup the joints were carefully designed so that both the top and the underside of the weld can be shielded.
Groove was selected as 70° as the thickness of the base metal was 2
Fig.1 V groove angle 5 Welding
In this experiment, the welding of titanium was carried out using thorium electrode. Welding is carried out on a C clamp arrangement on which titanium sheets are welded and welding parameters are considered.
Fig.2 Welding of Ti-6Al-4V sheets
Fig.3 Welded pieces of Ti-6Al-4V Table 1. Chemical composition of titanium
III.NON DESTRUCTIVE TESTING The main purpose of NDT is the detection of different material properties, especially non- homogeneities or defects, without mechanical damage of a tested object.
Methods of NDT USED
Most commonly used methods are:
1. Penetration testing 2. Radiography
Radiographic testing is a non destructive testing method of inspecting materials for hidden flaws by using the ability of short wavelength electromagnetic radiation to penetrate various materials. An x-ray machine can be used to detect the flaws in the specimen. Areas of the film exposed to less energy remain lighter.
Therefore, areas of the object where the thickness has been changed by discontinuities, such as porosity or cracks, will appear as dark outlines on the film.
Fig.4 Radiography testing equipment 2. Dye Penetrant
It is a widely applied and low-cost inspection method used to locate surface-breaking defects in all non-porous materials. In this method a liquid penetrant is applied to the surface of the product for a certain predetermined time, after which the excess penetrant is removed from the surface. The surface is then dried and a developer is applied to it. The penetrant which remains in the discontinuity is absorbed by the developer to indicate the presence as well as the location, size and nature of the discontinuity.
Table-2 Parameters taken into consideration while conducting DP
PARAMETER DESCRIPTION Material Titanium
method Visible, Solvent
removable Dwell time and
15 min at room temperature Acceptable standard ASTM-E-165 Developer M/s. The oriental
chemicals work Aluminu
oxygen titaniu m 6 Max
4 Max 0.2
3. TENSILE TESTING
Tensile testing is a fundamental test in which a sample is subjected to a controlled tension until failure. The most common testing machine used in tensile testing is the universal testing machine.
Fig.5 Tensile specimens of Ti-6Al-4V IV. RESULTS AND DISSCUSSION Table 3-Basic parameters noted while welding
Freq uenc ies
Ele ctro de
Peak Curr ent(I P)
Shi eldi ng Gas /
Base curr ent(I B)
We ld tim e Min
We ldi ng spe ed
86 10 40 2
pulse Tho riu m
90 10 39 1:3
89 10 35 2:2
pulse thor ium
86 10 40 1:2
5 Porosity and Cracks
According to the ASME SEC XI slandered with film size of 4o cm and focal spot size of 2 2
and density at about 1.8 to 3 / 3.Ti- 6Al-4V is given for radiography to check for flaws and detects if any. Finally the results showed that the test pieces are acceptable that means the flaws are within the acceptable limit.
Fig.6 X-Ray of the titanium gr-5 after radiography
Table 4 Radiography Test Results Sl.No. Pulsed/non
Frequency Physical observation
1 Non -
- No defect seen
2 Pulsed 2 No defect
3 Pulsed 4 Acceptable
4 Pulsed 6 Acceptable
5 Non -
6 Pulsed 2 Acceptable
7 Pulsed 4 No defect
8 Pulsed 6 No defect
seen Cracks in the Weldments
According to the ASTM E-1417 , the Dye- Penetrant (DP) test was conducted on these weldments. The test results are shown in table 12. The experimental results show that no cracks were observed in the weldments of this alloy in non-pulsed current and pulsed current welding.
Table – 5 Die penetration test results
Pulsed /non pulsed weldin
Frequ ency (Hz)
1 Non -
No defect observed on welded area
2 Pulsed 2 NDOWA
3 Pulsed 4 NDOWA
4 Pulsed 6 NDOWA
5 Non -
pulsed - NDOWA
6 Pulsed 2 NDOWA
7 Pulsed 4 NDOWA
8 Pulsed 6 NDOWA
Note : NDOWA-No defect observed on welded area
Table -6 Tensile test results Specimen
2 pulse sample no.1
640.6 843.5 3
2 pulse sample no.2
642.6 816.3 3
4 pulse sample no.1
768.7 887.5 3
4 pulse sample no.2
683.2 868.2 2
6 pulse sample no.1
630.9 804.2 2
6 pulse sample no.2
593.9 745.3 2
Non pulse sample no.1
509 645 1
Non pulse sample no.2
380 481.4 2
The tensile specimens were failed inside the weldments Non pulse and 6p (sample 2). The effeciency is calculated from ultimate tensile strength (UTS) of weldments in comparison to the base metal UTS. The results presented were best values obtained from two trails.
Effect of Current on Tensile Strength The Filler wire 4p produced maximum ultimate tensile strength i.e., 887.21Mpa. From the graph, it is observed that the ultimate tensile strength is more at frequency (4p)
Effect of Current on Yield Strength The Filler wire 4p produced maximum yield strength i.e., 768 . The various comparisons of current are shown in the table From the graph, it is observed that the yield strength is low at frequency (np).
Effect of Current on % of Elongation The effect of filler wire on % elongation is shown in Figure 4.5. From the graph, it is observed that at 2 pulse current has maximum
% of elongation when compared to the other currents .The maximum % of elongation value is 2.90. The maximum % of elongation produced at lower current because at lower current there are no much vibrations of torch and less heat produced when compared to higher current values.
From the experimental results, the following conclusions are drawn:
Porosity and Cracks
Results show that at 2 pulse two pores are present in the Welding area but they are within the acceptable limit of ASTM Standards. There are no surface cracks observed in he weld zone.
NP 2P 4P 6P S1 645 843 887 804 S2 481 816 868 745 5000
ULTIMATE TESILE STRENGTH
TENSILE TEST RESULTS
NP 2P 4P 6P
S1 509 640 768 630 S2 380 643 683 593 0
TENSILE TEST RESULTS
NP 2P 4P 6P
S1 0.54 2.9 2.36 1.86 S2 1.76 2.44 1.88 0.86 02
TENSILE TEST RESULTS
Ultimate tensile strength The 4 pulse produced maximum ultimate tensile strength.
The pulsed current has produced more tensile strength than non pulsed current.
The 4 pulse produced maximum yield strength.
The pulsed current has produced more yield strength than non pulsed current.
% of elongation
The 2 pulse has maximum % of elongation i.e., 2.90 %. The maximum % of elongation produced at lower current because at lower current there are no much vibrations of torch and less heat produced when compared to higher current values.
 Miller “Guidelines For Gas Tungsten Arc Welding”, TIG welding process, (2008), pp. 5-18
 A.Karpagaraj , N. Siva Shanmugam, K. Sankaranarayanasamy “The Effect Of Process Parameters On TIG Welding Of Thin Ti-6al-4v Sheets” Vol- 2, Issue- 10 Oct.-2014 International Journal of Mechanical And Production Engineering, ISSN: 2320-2092
 Wei Zhou and K.G. Chew, “Effect Of Welding On Impact Toughness Of Butt- Joints In A Titanium Alloy”, 2003 Materials science and engineering A, vol.
347, pp. 180-185
 S. Krishnanunni ,“Effect Of Welding Conditions On Hardness Of Commercially Pure Titanium”, July-Dec.
2012AKGEC International Journal of Technology, vol. 3, no. 2, pp. 19-24,.
 Yung, W. K.C., Ralph, B., Lee, W.B.
and Fenn, R, “An Investigation In To Welding Parameters Affecting The Tensile Properties Of Titanium Welds”, Journal of Materials Processing Technology, Vol. 63, (1997), pp. 759- 764
 B.H Choi, “The Effect Of Welding Conditions According To Mechanical Properties Of Pure Titanium”, May 2008.
Journal of Materials Processing Technology, vol. 201, issues 1–3, pp.526–530,
 N. Kishore Babu, S. Ganesh Sundara Raman, R. Mythili and S. Saroja,
“Correlation Of Microstructure With Mechanical Properties Of TIG
Weldments Of Ti–6Al–4V Made With And Without Current Pulsing”, 2007 Materials Characterization, vol. 58,issue 7, pp. 581–587,
 E. Ranatowski, ”Weldability Of Titanium And Its Alloys– Progress In Joining” University of Technology and Life Science, Mechanical Department St.
Prof. S.Kaliskiego 7, 85-763 Bydgoszcz, Poland DOI 10.2478/v10077-008-0033- 2: pp-70-76.
 Sicknan Soares da Rocha, Gelson Luis ADABO, Guilherme Elias Pessanha Henriques, Mauro Antonio de Arruda NOBILO “Vickers Hardness of Cast Commercially Pure Titanium and Ti- 6Al-4V Alloy Submitted to Heat Treatments” Braz Dent J pp:126-129  Vinicius A. R. Henrique’s,
“Titanium Production for Aerospace”
institute of Aeronautics and space Sao Jose dos Campos –Brazil pp: 1-16.
 T. S. Balasubramanian, M.
Balakrishnan, V. Balasubramanian M.A.Muthu Manickam, “Effect of welding processes on joint characteristics of Ti–6Al–4V alloy” Science and Technology of Welding and Joining stw 1922.3d 23/8/11 22:41:34 Vol No 1 PP:
 C. Casavola, F. Tattoli, C.
Pappalettere Politecnico di Bari,
“Static and Fatigue Characterization of Titanium Alloy Welded Joints”– Dip. di Ingegneria Meccanica e Gestionale.
 WA Baeslack III Ohio state university, J.R.Davis and associates, C.
E. Cross, martin Marietta Astronautics group, “Selection and weldability of conventional alloys” pp: 503-528.
 Paul Danielson, Rick Wilson and David Alman U. S. Department of Energy, Albany Research Center, Albany, Oregon “Microstructure of titanium welds”, 3/ 2004 February Edition 2003 of Advanced Materials and Processes pp:1-7.
 Bill Taylor, Struers Ltd, Glasgow Elisabeth Weidmann, Struers A/S, Copenhagen Metallographic preparation of Titanium Metals Handbook, Desk edition, ASM, 1984 p:
 Gh. R. Razavi1a, M. Masaeli1b, M.
Taheri2c, M. Saboktakin “Investigation gas tungsten arc welding of pure titanium” Department of Materials Engineering, Najafabad Branch, Islamic Azad University, Isfahan, P.O. Box 517, Iran International Journal of Materials and Mechanics Engineering, Vol. 2, No.
 J.Sieniawski, W. Ziaja, K. Kubiak and M. Motyka “Microstructure and Mechanical Properties of High Strength Two-Phase Titanium Alloys”
 Jian-wei MAO, Wei-jie LU, Li- qiang WANG, Di ZHANG, Ji-ning QIN “Microstructure and mechanical properties of GTA weldments of titanium matrix composites prepared with or without current pulsing” Received 22 May 2013; accepted 14 January 2014 pp:
 B.H. Choia, B.K. Choib, “The Effect Of Welding Conditions According To Mechanical Properties Of Pure Titanium” pp: 527-529
 www.arcam.com/wp-content/.../Arcam- Ti6Al4V-ELI-Titanium- Alloy.pd...
 “Titanium Alloy Guide” An Article of Rti International Metals, Inc.
 Arcam EBM system on Titanium Ti- 6Al-4V.